Please cite this article as: A. Salarvand, E. Poursaiedi, A. Azizpour, Probability Approach for Prediction of Pitting Corrosion Fatigue Life of Custom 450 Steel, International Journal of Engineering (IJE), IJE TRANSACTIONS A: Basics Vol. 31, No. 10, (October 2018) 1773-1781

## International Journal of Engineering

J o u r n a l H o m e p a g e : w w w . i j e . i r### Probability Approach for Prediction of Pitting Corrosion Fatigue Life of Custom 450

### Steel

A. Salarvanda_{, E. Poursaiedi*}b_{, A. Azizpour}b

*a _{Department of Mechanical Engineering, Islamic Azad University, Doroud Branch, Iran }*

*b*

_{ Department of Mechanical Engineering ,University of Zanjan, Zanjan, Iran }*P A P E R I N F O*

*Paper history: *

*Keywords*:
*Corrosion Fatigue *
*Corrosion Pit *
*Crack Propagation *
*High Cycle Fatigue *
*Custom 450 Steel*

*A B S T R A C T *

In this study, the pitting type of corrosion growth characteristics, fatigue crack initiation and
propagation behavior; axial fatigue tests were carried out on precipitation hardened martensitic Custom
450 steel in the air and 3.5wt% NaCl solution. Using the ratio of the depth to the half-width of the pits;
(a/c)= 1.5±0.2 the corrosion pit depth growth law was obtained as a function of stress amplitude and
elapsed time, t. Fatigue crack growth rates were determined in the near threshold stress intensity
factors regime (*∆kth*). A model was presented for estimation of corrosion fatigue life based on the time
to reach critical pit depth (as crack initiation) and crack propagation life. Then. S-N curves were
obtained both in air and NaCl solution from axial fatigue testing. Comparison of data from the
proposed model and the experimental results (S-N curves) showed good agreement.

**doi**: 10.5829/ije.2018.31.10a.21

**1. INTRODUCTION1**

Gas turbine compressor sections move large volumes of air that often contain significant amounts of airborne salt, water, and potentially corrosive gaseous species that can combine to form destructive acidic compounds. Precipitation-hardened martensitic Custom 450 stainless steel is used to make gas turbine compressor blades because it offers high strength, toughness and good corrosion resistance. Premature fracture failure in the first row of rotating blades of gas turbine compressors installed at a seaside power plant has been observed. Previous studies [1-3] revealed that the failure was caused by crack propagation from initial surface pitting that formed under a high cycle fatigue mechanism. The corrosion pits act as pre-existing flaws in the material to nucleate fatigue cracks.

Linear elastic fracture mechanics have been used in several investigations on durable cyclic loading in the presence of pitting corrosion [4-7]. The results of these models depend on the material and test conditions. Creating a relationship between pit size and elapsed

*Corresponding author E-mail: *epsaeidi@gmail.com* (E. Poursaeidi)

time in pit development has attracted a number of
studies. Sriraman et al. [8] developed a model that
considered the coexistence of a corrosive environment
and fatigue loading conditions and took into account the
influence of cyclic stress in pitting corrosion. Optical
profilometry and Weibull functions to characterize pit
depth and diameter distributions were used by
Cavanaugh and that found pit growth kinetics varied by
the environment, but most followed approximately *t*1/3
kinetics [9]. Sriraman proposed pit depth *ap as *
proportional to the cube root of *t * through the
relationship *ap=Bt1/3* [10].

Ishihara et al. [11] investigated corrosion pit growth
characteristics and fatigue crack initiation and
propagation behavior of the aluminum alloy 2024-T3 in
3% NaCl solution in detail. They developed a corrosion
pit growth law as a function of stress amplitude σa and
an elapsed time *t.* Shi and Mahadevan [12] studied the
damage tolerance approach for probabilistic pitting
corrosion fatigue life prediction and found that pit
nucleation time and the material constant for short crack
growth (*∆kth) are the two most important random *
variables affecting corrosion fatigue life.
Bastidas-Arteaga [13] developed a model to predict corrosion
fatigue lifetime. The results showed that the coupled
Received 10 November 2017

A. Salarvand et al. / IJE TRANSACTIONS A: Basics Vol. 31, No. 10, (October 2018) 1773-1781 1774

effect of corrosion and fatigue on a structure strongly affects performance and can significantly decrease the expected lifetime.

Lin and Tsai [14] evaluated corrosion fatigue behavior of a 15Cr–6Ni Custom 450 steel under three different aging conditions to characterize the effects of aging treatment on corrosion fatigue (CF) resistance in laboratory air and 3.5 wt% NaCl solutions. Fatigue resistance in all three tempers decreased dramatically in the aqueous NaCl environment according to S–N results. In addition, it was found that the peak-aged steel temper exhibited highest CF resistance while, the over-aged sample had the lowest value. Some authors [15, 16] have dealt with fatigue life estimation of pitted 12% Cr steel using the short crack approach [17] to estimate the durable cyclic stress according to pit size.

Additional research [18-24] has been conducted on pitting corrosion fatigue in various materials, but none thus far have examined the growth of pits and transition from pit to crack in C450 steel. Following previous investigations by the authors, the present study focuses on the mechanism of growth of corrosion pits under the cyclic loading and prediction of corrosion fatigue life using the corrosion pit growth law for Custom 450 steel.

**2. MATERIALS AND METHODS **

**2. 1. Materials **Samples of Custom 450 steel were
prepared by cutting and machining of scrap blades of a
gas turbine compressor. The results of quantometery
and chemical analysis of a sample of the materials are
shown in Table 1. This type of steel was heated at 1030
°C for 0.5 h and then was quenched in water.
Precipitation hardening was then carried out at 530 °C
(1050 °F) for 4 h [25] to obtain a microhardness of
310±10 HV. The mechanical properties of the material
are shown in Table 2.

**TABLE 1.** Chemical analysis of C450 stainless steel

**Element ** **Wt (%) **

C 0.027

Mn 0.6

Si 0.245

P 0.0166

Co 0.0604

Cr 15.17

Ni 6.43

Mo 0.79

Cu 1.48

Nb 0.35

Fe Blance

**TABLE 2.** Mechanical properties of Custom 450 at room

temperature (provided by the supplier)

**Tensile strength **
**(MPa) **

**Yield strength **
**(MPa) **

**Elongation A **
**(%) **

**Hardness **
**(HV) **

1100 1060 21 310

**Figure 1.** Specimens used to test: (a) fatigue (S-N) and; (b)
FCGR. All dimensions are in mm

**2. 2. Test Sample Preparation **Twenty-five
fatigue specimens were made according to ASTM E466
standards [26] for fatigue testing and measurement of
corrosion pit dimensions (Figure 1(a)). Also six
specimens were prepared to measure fatigue crack
growth rate (FCGR) (Figure 1(b)). The sample surfaces
were initially machined and then ground and polished
using grade 400 to 4000 abrasive papers. The surfaces
were fully polished and mirrored using cloth and fluids
with abrasive nano-silica particles. Plate-shaped
samples with a starter notch were used to measure
FCGR and to determine the threshold stress intensity
factor (Figure 1(b)). A hole 2 mm in diameter was
drilled in the middle of the sample then a groove crack
0.35 mm wide and 2 mm length was created by
electrical discharge machining on one side of the hole.

**3. TESTING PROCEDURES **

**3. 1. Corrosion Pit Depth Measurement Under **
**Cyclic Loading **An axial fatigue testing machine
was used to produce the Corrosion Fatigue (CF) pits.
During the pitting and corrosion fatigue tests, samples
were placed in a solution of 3.5% wt NaCl under cyclic
loading in the form of a sine wave at a frequency of 20
Hz and stress ratio of R = 0.1 at stress amplitudes of 0,
150, 250, 300 and 325 MPa.

the surface of the polymer material and the effects of pits and surface roughness of the sample remain on the surface of the polymer material in raised relief (Figure 3).

The surface topography of the samples was
produced using Repliset method and CF tests were
carried out on the samples. After specified periods of
time, testing was halted and the sample surface features
were again recorded and the test continued. The height
of Repliset relief patterns represent the depth of the
corrosion pits and were measured using the focused
focal point method. The diameter of the relief on the
surface of Repliset was measured and found to be
equivalent to pit diameter. The time variations of the
maximum pit depth distribution were then measured. A
portion of the sample surface 14.4 mm2_{ in the area (right }
image of Figure 4) was divided into 12 parts, each 1.2
mm2_{ in area. In order to better observation of micro pits, }
12 images were taken on each area (left image of Figure
4). The biggest pit was determined in each area and its
dimensions measured.

**3. 2. Fatigue Tests **Axial tests based on ASTM
E466 were carried out on a servo hydraulic fatigue test
machine to determine the S-N curves at a constant sine
stress amplitude at a frequency of 20 Hz with a stress
ratio of R = 0.1 at room temperature. Measurement of
FCGR began at a frequency of 20 Hz (55Mpa*< σ < *550
Mpa*; *R = 0.1) with a high crack growth rate of (10-8
10-9_{) m/cycle. After crack advance was detected with the }
length of 1mm, Δ*k* was gradually decreased and this
process was repeated until crack growth arrested. The
lowest value recorded for Δ*k* was considered as Δ*kth.*

**4. TEST RESULTS **

**4. 1. Corrosion Pits Formation During Corrosion **
**Fatigue **Figure 5 shows images of corrosion pit
formation taken by an optical microscope under cyclic
loading at a stress amplitude of σa = 250 MPa and stress
ratio of R = 0.1. The figure shows pit formation of the
sample surface before the test and after 3 and 6 h of
testing. As seen, the size and number of the pits
increased as the time increased.

(a) (b)

**Figure 2.** Fatigue testing machine: (a) Running the corrosion
fatigue test; (b) corrosion cell

**Figure 3. **SEM surface views of Replisets

**Figure 4.** Surface view divided into 12 parts and 12

photographs of the parts

**Figure 5. **Successive images of corrosion pits during CF

testing (*σa *= 250 MPa, R= 0.1, *f *= 20 Hz): (a) before testing (*t *
= 0); (b) *t *= 3 h; (c) *t* = 6 h

**4. 2. Time Versus Maximum Pit Depth **
**Distribution **Studies have shown that it is difficult
to determine the exact behavior and growth of corrosion
pits. The pits that have the same diameter and depth do
not necessarily grow in a similar fashion. One reason for
this is that measurement of pit dimensions is influenced
by individual characteristics such as choice of the pit
and by observations made. For this reason, the
variations in pit formation over time was investigated as
maximum pit depth distribution.

A. Salarvand et al. / IJE TRANSACTIONS A: Basics Vol. 31, No. 10, (October 2018) 1773-1781 1776

distribution was plotted to obtain the maximum pit
depth distribution. Figure 6 shows time versus the
maximum pit depth distribution plotted on the largest
extreme-value. The data was plotted at stress amplitudes
of 0, 150, 250, 300 and 325 MPa. As the figure shows,
the distribution of the maximum pit depth moved to the
right as time increased, indicating pit depth increased as
time increased. It was also observed that the maximum
pit depth distribution was linear, which means that the
distribution of the maximum pit depth (*ai*) can be
expressed as a double exponential relationship as
follows:

(1)

where µ denotes scale and α denotes location parameter.

**4. 3. Effect of Stress Amplitude on the Time**
**Variation of the Distribution of the Maximum Pit **
**Depth ** Figure 7 shows the distribution of the
maximum pit depth, *F(ai)*, for amplitudes of 150, 250,
300 and 325 MPa with constant elapsed time to clarify
the effect of stress amplitude on the time variation of the
distribution, *F(ai)*. As seen, the growth rate of the pits
increased as the stress amplitude increased. The effect
of stress amplitude on the growth rate of pit depth is
apparent. To investigate the effect of elapsed time on
the maximum pit depth distribution, location parameter
(α) in Equation (1) from Figure 8 was used. By plotting
the log-log curve for α versus time (*t*) for different stress
amplitudes, variations in α according to stress amplitude
can be determined (Figure 8).

**4. 4. Corrosion Pit Growth Formulation **The test
results show that the growth rate of corrosion pit depth
is affected by cyclic stress amplitude. Results of the

previous research have shown that the effect of loading frequency on corrosion pit growth is insignificant [11]. So far, Equation (2) was used as a corrosion pit growth law [7]:

(2)

where *a* is corrosion pit depth, *t* is the elapsed time and
*A* and *β* are constants determined by testing. Because
stress amplitude σa effects on corrosion pit growth, it
should be considered in the equation in addition to
elapsed time (t). Equation (2) has been modified to
include stress amplitude as:

(3)

where *A*(*σa) is the stress amplitude function and β *is the
power index of time. Location parameter α for
maximum pit depth distribution was used instead of
corrosion pit depth (*a*), because this parameter
represents the highst density of data which can be
extracted for maximum pit depth estimation in
extreme-value theory. The extreme-values for *A(σa)* and *β* in Equation (3)
were obtained by calculating the gradient and intercept
of the lines in Figure 8 and are shown in Table 3.

By averaging the values for *β* for different stress
amplitudes, a value of 0.34 was determined. Using a
log-normal plot of the *A*(*σa) values versus * *σa and *
measuring the resulting gradient and intercept (Figure 9)
produces Equation (4) for *A*(*σa). Corrosion pit growth *
law is expressed in Equation (5):

(4)

(5)

where *a* (μm), *σa (MPa) and t* (h) are pit depth, cyclic
stress amplitude and elapsed time, respectively.m

**Figure 7. **Maximum pit depth distribution (*F(ai)*) for amplitudes of 150, 250, 300 and 325MPa at *t* = 1 h and *t* = 6 h

**4. 5. Geometric Characteristics of Pits **Scanning
electron microscopy (SEM) and optical microscopy of
the specimen surfaces under CF showed that most pits
were irregular in shape and that pits had different
geometries; however, they can be assumed to be
roughly semi-elliptical (Figure 10). Measurement of pit
dimensions showed that the ratio of the depth to the
half-width of the pits can be expressed as: a/c = 1.5 ±
0.2. Cross-sections of pits that were initially circular
were shown to become elliptical gradually under the
applied stress, particularly when the stress concentration
occurred on both sides.

**4. 6. Crack Initiation Criteria **It has been proven
that cracks initiate from corrosion pits which arise
during CF [20, 21]. To determine the status of crack
initiation from a corrosion pit, CF tests were conducted
using axial loading on the flat samples. The assumption
that pits at the threshold of cracking will behave like
cracks is not uncommon. Several relationships have
been suggested to calculate the threshold stress intensity
factor based on pit dimension using linear elastic
fracture mechanics (LEFM). One example is:

(6)

where *∆Kth is the threshold stress intensity factor range, *

*∆σth is the threshold fatigue strength range, a *is the

depth of the pit and *γ* is a geometrical factor equal to
0.67 for semicircle surface cracks [5, 22].

Murakami [23] used Equation (7) to calculate the
critical stress intensity factor for crack initiation when
pits become crack (*∆Kpit→areak)* of irregular surface
cracks as:

(7)

where Δ*σ* is the range of applied tensile stress and

*areap→c is the pit cross-section in the direction *

perpendicular to the applied tensile load. Assuming that
the value of *∆Kp→c = ∆Kth, areap→c can be calculated for *
different stress amplitudes. The value of *∆Kth can be *
obtained from the FCGR curve. Assuming that critical

pit depth *ath equals* , Equation (5) can be used
to calculate the time required to reach critical pit depth
and crack initiation for each stress amplitude.

**Figure 8. **Effect of stress amplitudes on the relationship

between location parameter αand an elapsed time, *t*

**TABLE 3**. Values of *A*(*σa*) and *β* for each stress amplitude

**Stress Amplitude (σa ) (MPa) ** **A(σa) ** **β **

0 3.861 0.338

150 7.471 0.340

250 11.272 0.352

300 14.588 0.338

325 16.865 0.356

A. Salarvand et al. / IJE TRANSACTIONS A: Basics Vol. 31, No. 10, (October 2018) 1773-1781 1778

**Figure 10. **Generalschematic fracture surface including a pit

**4. 7. Determination of FCGR Curves in Air and **
**Saline Solution **FCGR measurement was carried
out in the near-threshold regime at a stress ratio of R =
0.1. Testing was done in both air and a solution of 3.5%
wt NaCl. Figure 11 shows the two FCGR curves. The
threshold stress intensity factor range (*∆Kth)*

### ,

where the crack growth rate is less than### ,

for the saline environment and air were 3.3 and 3.8 MPa , respectively. As seen from the figure, the general relationship according to the Paris equation takes the form:(8)

where *a* and *∆K are the depth of the crack and the stress *
intensity factor range, respectively, and *C* and *m* are
material constants.

Assuming that the shape of the pit is semi-ellipsoidal, Equation (9) can be used to calculate the stress intensity factor [24] as:

,

(9)

Assuming that *c*/*a* = 0.667, the stress intensity factor
becomes:

(10)

**4. 8. S-N Tests **Axial fatigue test data and S-N
curves in the air and saline solution are shown in Figure
12 at a frequency of 20 Hz and a stress ratio of R = 0.1
for smooth and polished samples.The tests continued to
failure the samples. The results show that the material
fatigue strength decreased in the corrosive
environments. The maximum stress applied to the
sample at 555 to 930 MPa (0.5 to 0.85 σu) changed
according to the sample and environmental condition.
The solid lines in Figure 12 denote the testing data for
which the following parametric relation can be
considered:

(11)

where *S* is the maximum alternative stress, *Nf* is the
number of failure cycles, is the fatigue strength
coefficient, and *n* is the fatigue exponent. Table 4
summarizes the values of and *n. *

**5. DISCUSSION **

**5. 1. Estimation of Crack Initiation Life **Using
relation *N* = *ft* between the number of stress cycles *N*
and time *t* which *f* is the cyclic stress frequency and
combining it with Equation (5) produces crack initiation
life (*Ni) as:*

(12)

Substituting obtained from the

FCGR curve for the 3.5% wtNaCl solution environment

and and assuming results

in:

(13)

Substituting Equation (13) into Equation (7) produces:

(14)

Now *ath can be obtained for any range of stress ∆σ* from

Equation (14) and, by substituting it into Equation(12),
crack initiation life *Ni can be calculated as the critical *
pit life.

**Figure 11. **FCGR curves for cracks emanating from pits in the

air and 3.5% NaCl solution

**TABLE 4**. Parameters used in Equation (11)

**n**** (MPa)**

**Material & test environment **

-0.0798 2142.9

C450- in air

-0.1078 2666.8

**Figure 12.** S-N curves in air and 3.5 wt% NaCl solution

**5. 2. Estimation of Crack Growth Life **With
substituting Equation (10) in to the Equation (8) and
integration from *ath * (critical pit depth) to
(*w* width of the sample), crack
propagation life *Np becomes:*

(15)

Corrosion fatigue life *Nf is estimated to be the sum of *
crack initiation life *Ni and crack propagation life Np. *

**5. 3. Validation of Corrosion Fatigue Model **In
order to evaluate the accuracy of the prediction for
results of the presented model, fractographic images of
the fracture surface of a number of specimens (that
failed during CF testing used to determine the S-N
curves) were analyzed by SEM. Figure 13 shows
fracture surface of a test sample in a solution of 3.5% wt
NaCl for which *σmax = 667 MPa and R = 0.1 at 20 Hz *
frequency that failed after 472,351 cycles. The source of
crack initiation is determined by the convergence of the
fracture marking lines. As the figure indicates, the

critical pit cross-section is and *ath = *

24 µm.

In the proposed model, by assuming

from the FCGR curve for this material, the critical cross-section of the pit for stress

range Δ*σ* = 600 MPa equals ,

and, thus, , and

cycles. This represents about a %10 deviation from the test results (472,351 cycles).

Figure 14 compares the tests results and the estimated corrosion fatigue life from the proposed model. As seen, the estimated results are in good agreement with the experimental data, although estimations show a shorter life span than the experimental results. This may have resulted from the absence of consideration of the onset time (before the formation of the pit) of the initial pit.

**Figure 13.** The fracture surface of the test sample in 3.5%wt
NaCl solution and the cross-section area of the pit

**Figure 14. ** Comparison of estimated and experimental

corrosion fatigue life

With a decrease in stress amplitude, the corrosion pit growth rate decreased, the time span of crack initiation increased and CF life also increased. At low stress amplitudes, most CF life relates to the growth of the corrosion pit. This is why a complete understanding of the growth mechanisms of a corrosion pit is important for fatigue life assessment.

**6. CONCLUSION **

The present study investigated pitting corrosion fatigue behavior of precipitation hardened Custom 450 steel using tensile axial fatigue testing at a 3.5% wt NaCl solution. Fatigue crack growth characteristics and the behavior of fatigue pit initiation and its propagation were evaluated. Measurement of the fatigue crack growth rate (FCGR) near the threshold regime and S-N tests in the high cycle regime was conducted on perfectly smooth samples in air and 3.5%wt NaCl solution. The results are summarized below.

1. Corrosion pit depth (µm) can be presented as a function of stress amplitude (MPa) and elapsed time

(h) as .

A. Salarvand et al. / IJE TRANSACTIONS A: Basics Vol. 31, No. 10, (October 2018) 1773-1781 1780

critical stress intensity factor for crack initiation
*∆kp→c* from the corrosion pit.

3. Crack propagation life in saline solution was calculated using the relationship

from the FCGR curve. Corrosion fatigue life *Nf*can
be calculated as the sum of crack initiation life (*Ni; *
calculated using the law of corrosion pit growth
under critical conditions) and crack propagation life
(*Np). *

4. Results of the proposed model and the relationships used to determine the corrosion fatigue life were in good agreement with the experimental results on the S-N curve.

5. The S-N curves showed that the fatigue limit in the saline solution was less than in air and this difference was more evident at lower stress amplitudes. At the low stress amplitudes, the corrosion pit growth was primarily related to fatigue life.

7. **REFRENCES **

1. Poursaeidi, E., Sanaieei, M., and Bakhtyari, H., “Life Estimate
of a Compressor Blade through Fractography”, **International *** Journal of Engineering - Transactions A: Basics*, Vol. 26, No.
4, (2012), 393–400.

2. Poursaeidi, E., Babaei, A., Behrouzshad, F., and Mohammadi
Arhani, M.R., “Failure analysis of an axial compressor first row
rotating blades”, * Engineering Failure Analysis*, Vol. 28,
(2013), 25–33.

3. Poursaeidi, E., and Pedram, O., “An Outrun Competition of
Corrosion Fatigue and Stress Corrosion Cracking on Crack
Initiation in a Compressor Blade”, **International Journal of *** Engineering - Transactions B: Applications*, Vol. 27, No. 5,
(2013), 785–792.

4. Lindley, T.C., Mcintyre, P., and Trant, P.J., “Fatigue-crack
initiation at corrosion pits”, * Metals Technology*, Vol. 9, No. 1,
(1982), 135–142.

5. Kondo, Y., “Prediction of fatigue crack initation life based on pit
growth”, * Corrosion*, Vol. 45, No. 1, (1989), 7–11.

6. Kawai, S., and Kasai, K., “Considerations of Allowable Stress of Corrosion Fatigue (Focussed on the Influence of Pitting)”,

* Fatigue & Fracture of Engineering Materials & Structures*,
Vol. 8, No. 2, (1985), 115–127.

7. Turnbull, A., McCartney, L.N., and Zhou, S., “A model to
predict the evolution of pitting corrosion and the pit-to-crack
transition incorporating statistically distributed input
parameters”, * Corrosion Science*, Vol. 48, No. 8, (2006), 2084–
2105.

8. Sriraman, M.R., and Pidaparti, R.M., “Crack Initiation Life of
Materials Under Combined Pitting Corrosion and Cyclic
Loading”, * Journal of Materials Engineering and Performance*,
Vol. 19, No. 1, (2010), 7–12.

9. Cavanaugh, M., Buchheit, R., and Birbilis, N., “Modeling the
environmental dependence of pit growth using neural network
approaches”, * Corrosion Science*, Vol. 52, No. 9, (2010), 3070–
3077.

10. Sriraman, M.R., and Pidaparti, R.M., “Life Prediction of Aircraft

Aluminum Subjected to Pitting Corrosion Under Fatigue
Conditions”, * Journal of Aircraft*, Vol. 46, No. 4, (2009), 1253–
1259.

11. Ishihara, S., Saka, S., Nan, Z.Y., Goshima, T., and Sunada, S.,
“Prediction of Corrosion Fatigue Lives of Aluminium Alloy on
The Basis of Corrosion Pit Growth Law”, **Fatigue and Fracture *** of Engineering Materials and Structures*, Vol. 29, No. 6,
(2006), 472–480.

12. Shi Pan, M.S., “Damage tolerance approach for probabilistic
pitting corrosion fatigue life prediction”, **Engineering Fracture *** Mechanics*, Vol. 68, No. 13, (2001), 1493–1507.

13. Bastidas-Arteaga, E., Bressolette, P., Chateauneuf, A., and
Sánchez-Silva, M., “Probabilistic lifetime assessment of RC
structures under coupled corrosion–fatigue deterioration
processes”, * Structural Safety*, Vol. 31, No. 1, (2009), 84–96.
14. Lin, C.K., and Tsai, W.J., “Corrosion fatigue behaviour of a

15Cr-6Ni precipitation-hardening stainless steel in different
tempers”, **Fatigue and Fracture of Engineering Materials and *** Structures*, Vol. 23, No. 6, (2000), 489–497.

15. Schonbauer, B.M., Stanzl-Tschegg, S.E., Perlega, A., Salzman, R.N., Rieger, N.F., Zhou, S., Turnbull, A., and Gandy, D., “Fatigue life estimation of pitted 12% Cr steam turbine blade steel in different environments and at different stress ratios”,

* International Journal of Fatigue*, Vol. 65, (2014), 33–43.
16. Schonbauer, B.M., Perlega, A., Karr, U.P., Gandy, D., and

Stanzl-Tschegg, S.E., “Pit-to-crack transition under cyclic loading in
12% Cr steam turbine blade steel”, **International Journal of *** Fatigue*, Vol. 76, (2015), 19–32.

17. El Haddad, M.H., Topper, T.H., and Smith, K.N., “Prediction of
non propagating cracks”, * Engineering Fracture Mechanics*,
Vol. 11, No. 3, (1979), 575–584.

18. Lindström, R., Johansson, L., Thompson, G., Skeldon, P., and Svensson, J.E., “Corrosion of magnesium in humid air”,

* Corrosion Science*, Vol. 46, No. 5, (2004), 1141-1158.
19. Harlow, D.G., and Wei, R.P., “A probability model for the

growth of corrosion pits in aluminum alloys induced by
constituent particles”, * Engineering Fracture Mechanics*, Vol.
59, No. 3, (1998), 305–325.

20. Medved, J.J., Breton, M., and Irving, P.E., “Corrosion pit size
distributions and fatigue lives—a study of the EIFS technique
for fatigue design in the presence of corrosion”, **International *** Journal of Fatigue*, Vol. 26, No. 1, (2004), 71–80.

21. Xie J., Alpas A.T., Northwood D.O., “A mechanism for the
crack initiation of corrosion fatigue of Type 316L stainless steel
in Hank’s solution”, * Materials Characterization*, Vol. 48, No. 4,
(2002), 271–277.

22. Ishihara, S., McEvily, A.J., and Shiozawa, K., “A
fatigue‐crack‐growth‐based analysis of two‐step corrosion
fatigue tests”, **Fatigue and Fracture of Engineering Materials *** and Structures*, Vol. 18, No. 11, (1995), 1311–1321.

23. Murakami, Y., “Metal Fatigue: Effects of Small Defects and Nonmetallic Inclusions”, Elsevier, (2002).

24. Hayashi, K., and Abe, H., “Stress intensity factors for a semi-elliptical crack in the surface of a semi-infinite solid”,

* International Journal of Fracture*, Vol. 16, No. 3, (1980), 275–
285.

25. Kosa, T., and DeBold, T., “Effect of Heat Treatment and Microstructure on the Mechanical and Corrosion Properties of a Precipitation Hardenable Stainless Steel”, In MiCon 78: Optimization of Processing, Properties, and Service Performance Through Microstructural Control, ASTM International, (1979), 367–392.

### Probability Approach for Prediction of Pitting Corrosion Fatigue Life of Custom 450

### Steel

A. Salarvanda_{, E. Poursaiedi}b_{, A. Azizpour}b

*a _{Department of Mechanical Engineering, Islamic Azad University, Doroud Branch, Iran }*

*b*

_{ Department of Mechanical Engineering ,University of Zanjan, Zanjan, Iran }*P A P E R I N F O*

*Paper history: *

Received 10 November 2017 Received in revised form 09 june 2018 Accepted 17 August 2018

*Keywords*:
*Corrosion Fatigue *
*Corrosion Pit *
*Crack Propagation *
*High Cycle Fatigue *
*Custom 450 Steel*

**هدیکچ**

نومزآ ،دشر راتفر و یگتسخ کرت عورش ،یگدروخ هرفح دشر تاصخشم یبایزرا تهج ،هعلاطم نیا رد یگتسخ یاه

هدش یتخس بوسر یتیزنترام دلاوف یور رب یروحم Custom 450

لولحم و اوه رد

5

/

3

دصرد NaCl دش ماجنا رد اب .

ع فصن هب قمع تبسن نتفرگ رظن هرفح ضر

تروصب اه ،

یعبات ناونع هب یگدروخ هرفح قمع دشر نوناق

شنت هنماد زا

a σ هدش یرپس نامز و t

.دش هدز نیمخت خرن

کیدزن یحاون رد یگتسخ کرت دشر یاه روتکاف

شنت تدش

ارحب قمع هب ندیسر نامز ساسا رب یگدروخ یگتسخ رمع نیمخت یارب یلدم و دندش نییعت هناتسآ دشر رمع و هرفح ین

ینحنم سپس .دش هئارا کرت یاه

S-N شیامزآ زا لولحم و اوه رد یروحم یگتسخ یاه NaCl

هسیاقم هک دندمآ تسدب

هداد ینحنم( یهاگشیامزآ جیاتن اب یداهنشیپ لدم یاه یاه

S-N .داد ناشن ار یبوخ قفاوت )